Download presentation

Presentation is loading. Please wait.

1
Talk online at http://pantheon.yale.edu/~subir Eugene Demler (Harvard) Kwon Park Anatoli Polkovnikov Subir Sachdev Matthias Vojta (Augsburg) Ying Zhang Order and quantum phase transitions in the cuprate superconductors

2
Mott insulator: square lattice antiferromagnet Parent compound of the high temperature superconductors: Ground state has long-range magnetic Néel order, or a “spin density wave (SDW)” Néel order parameter:

3
Introduce mobile carriers of density by substitutional doping of out-of-plane ions e.g. Exhibits superconductivity below a high critical temperature T c

4
low Several low temperature properties of the cuprate superconductors appear to be qualitatively similar to those predicted by BCS theory. Bose-Einstein condensation of Cooper pairs

5
Superconductivity in a doped Mott insulator Hypothesis: cuprate superconductors are characterized by additional order parameters, associated with the proximate Mott insulator, along with the familiar order associated with the Bose condensation of Cooper pairs in BCS theory. These orders lead to new low energy excitations. Predictions of BCS associated with underlying Fermi surface do not apply Review: S. Sachdev, Science 286, 2479 (1999).

6
Superconductivity in a doped Mott insulator Study physics in a generalized phase diagram which includes new phases (which need not be experimentally accessible) with long- range correlations in the additional order parameters. Expansion away from quantum critical points provides a systematic and controlled theory of the low energy excitations (including their behavior near imperfections such as impurities and vortices and their response to applied fields) and of crossovers into “incoherent” regimes at finite temperature. Review: S. Sachdev, Science 286, 2479 (1999).

7
Outline I.What is a quantum phase transition ? II.The simplest quantum phase transition Quantum Ising Chain III.Coupled Ladder Antiferromagnet IV.A global phase diagram V.Recent neutron scattering and STM experiments on the cuprates. VI.Conclusions I. What is a quantum phase transition ?

8
What is a quantum phase transition ? Non-analyticity in ground state properties as a function of some control parameter g E g True level crossing: Usually a first-order transition E g Avoided level crossing which becomes sharp in the infinite volume limit: second-order transition

9
T Quantum-critical Critical excitations control dynamics in the wide quantum-critical region at non-zero temperatures. No collective classical variables for large scale dynamics. Why study quantum phase transitions ? Theory for a quantum system with strong correlations: describe phases on either side of g c by expanding in deviation from the quantum critical point. g gcgc Important property of ground state at g=g c : temporal and spatial scale invariance; characteristic energy scale at other values of g: Critical point is a novel state of matter without quasiparticle excitations

10
Outline I.What is a quantum phase transition ? II.The simplest quantum phase transition Quantum Ising Chain III.Coupled Ladder Antiferromagnet IV.A global phase diagram V.Recent neutron scattering and STM experiments on the cuprates. VI.Conclusions II. The simplest quantum phase transition

11
I. Quantum Ising Chain 2Jg

12
Full Hamiltonian leads to entangled states at g of order unity

13
Weakly-coupled qubits Ground state: Lowest excited states: Coupling between qubits creates “flipped-spin” quasiparticle states at momentum p Entire spectrum can be constructed out of multi-quasiparticle states p

14
Ground states: Lowest excited states: domain walls Coupling between qubits creates new “domain- wall” quasiparticle states at momentum p p Strongly-coupled qubits

15
Entangled states at g of order unity g gcgc “Flipped-spin” Quasiparticle weight Z A.V. Chubukov, S. Sachdev, and J.Ye, Phys. Rev. B 49, 11919 (1994) g gcgc Ferromagnetic moment N 0 P. Pfeuty Annals of Physics, 57, 79 (1970) g gcgc Excitation energy gap

16
Quasiclassical dynamics S. Sachdev and J. Ye, Phys. Rev. Lett. 69, 2411 (1992). S. Sachdev and A.P. Young, Phys. Rev. Lett. 78, 2220 (1997). Crossovers at nonzero temperature

17
Outline I.What is a quantum phase transition ? II.The simplest quantum phase transition Quantum Ising Chain III.Coupled Ladder Antiferromagnet IV.A global phase diagram V.Recent neutron scattering and STM experiments on the cuprates. VI.Conclusions III. Coupled ladder antiferromagnet

18
S=1/2 spins on coupled 2-leg ladders II. Coupled Ladder Antiferromagnet N. Katoh and M. Imada, J. Phys. Soc. Jpn. 63, 4529 (1994). J. Tworzydlo, O. Y. Osman, C. N. A. van Duin, J. Zaanen, Phys. Rev. B 59, 115 (1999). M. Matsumoto, C. Yasuda, S. Todo, and H. Takayama, Phys. Rev. B 65, 014407 (2002).

19
Square lattice antiferromagnet Experimental realization: Ground state has long-range magnetic (Neel) order Excitations: 2 spin waves

20
Weakly coupled ladders Paramagnetic ground state Spin gap Real space Cooper pairs with their charge localized. Upon doping, motion and Bose-Einstein condensation of Cooper pairs leads to superconductivity

21
Excitations Excitation: S=1 exciton (spin collective mode) Energy dispersion away from antiferromagnetic wavevector Spin gap S=1/2 spinons are confined by a linear potential.

22
1 c Quantum paramagnet Electrons in charge-localized Cooper pairs Neel state Magnetic order as in La 2 CuO 4 Neel order N 0 Spin gap T=0 in cuprates

23
Spin gap Paramagnetic ground state of coupled ladder model

24
Spin gap Can this be a paramagnetic ground state of a system with full square lattice symmetry ? Such a state breaks lattice symmetry by the appearance of bond order Such bond order is generic in paramagnetic states proximate to a magnetic state with collinear spins N. Read and S. Sachdev, Phys. Rev. Lett. 62, 1694 (1989).

25
Origin of bond order Quantum “entropic” effects prefer bond-ordered configurations in which the largest number of singlet pairs can resonate. The state on the upper left has more flippable pairs of singlets than the one on the lower left. These effects lead to a broken square lattice symmetry near the transition to the magnetically ordered states with collinear spins.

26
Outline I.What is a quantum phase transition ? II.The simplest quantum phase transition Quantum Ising Chain III.Coupled Ladder Antiferromagnet IV.A global phase diagram V.Recent neutron scattering and STM experiments on the cuprates. VI.Conclusions IV. A global phase diagram

27
Order parameters in the cuprate superconductors 1. Pairing order of BCS theory Bose-Einstein condensation of Cooper pairs Orders associated with proximate Mott insulator 2. Collinear magnetic order 3. Bond order For most wavevectors, these orders also imply a modulation in the site charge density (“charge order”). However, the amplitude of the charge order should be strongly suppressed by Coulomb interactions. S. Sachdev and N. Read, Int. J. Mod. Phys. B 5, 219 (1991).

28
Doping a paramagnetic bond-ordered Mott insulator Systematic Sp(N) theory of translational symmetry breaking, while preserving spin rotation invariance. S. Sachdev and N. Read, Int. J. Mod. Phys. B 5, 219 (1991). Instability to phase separation below this line d-wave superconductor Superconductor with co-existing bond-order Mott insulator with bond-order T=0

29
IV. A global phase diagram Include long-range Coulomb interactions: frustrated phase separation V.J. Emery, S.A. Kivelson, and H.Q. Lin, Phys. Rev. Lett. 64, 475 (1990). M. Vojta and S. Sachdev, Phys. Rev. Lett. 83, 3916 (1999) M. Vojta, Y. Zhang, and S. Sachdev, Phys. Rev. B 62, 6721 (2000). M. Vojta, Phys. Rev. B 66, 104505 (2002). See also J. Zaanen, Physica C 217, 317 (1999), S. White and D. J. Scalapino, Phys. Rev. Lett. 80, 1272 (1998). C. Castellani, C. Di Castro, and M. Grilli, Phys.Rev. Lett. 75, 4650 (1995). S. Mazumdar, R.T. Clay, and D.K. Campbell, Phys. Rev. B 62, 13400 (2000). Collinear magnetic order Bond order

30
Outline I.What is a quantum phase transition ? II.The simplest quantum phase transition Quantum Ising Chain III.Coupled Ladder Antiferromagnet IV.A global phase diagram V.Recent neutron scattering and STM experiments on the cuprates. VI.Conclusions V. Recent neutron scattering and STM experiments on the cuprates

31
kyky kxkx /a 0 Insulator ~0.12-0.14 0.055 SC 0.020 J. M. Tranquada et al., Phys. Rev. B 54, 7489 (199 6). G. Aeppli, T.E. Mason, S.M. Hayden, H.A. Mook, J. Kulda, Science 278, 1432 (1997). S. Wakimoto, G. Shirane et al., Phys. Rev. B 60, R769 (1999). Y.S. Lee, R. J. Birgeneau, M. A. Kastner et al., Phys. Rev. B 60, 3643 (1999) S. Wakimoto, R.J. Birgeneau, Y.S. Lee, and G. Shirane, Phys. Rev. B 63, 172501 (2001). (additional commensurability effects near =0.125) T=0 phases of LSCO V. Tuning magnetic order in LSCO by a magnetic field SC+SDW SDW Néel

32
kyky kxkx /a 0 Insulator ~0.12-0.14 0.055 SC 0.020 J. M. Tranquada et al., Phys. Rev. B 54, 7489 (199 6). G. Aeppli, T.E. Mason, S.M. Hayden, H.A. Mook, J. Kulda, Science 278, 1432 (1997). S. Wakimoto, G. Shirane et al., Phys. Rev. B 60, R769 (1999). Y.S. Lee, R. J. Birgeneau, M. A. Kastner et al., Phys. Rev. B 60, 3643 (1999) S. Wakimoto, R.J. Birgeneau, Y.S. Lee, and G. Shirane, Phys. Rev. B 63, 172501 (2001). (additional commensurability effects near =0.125) T=0 phases of LSCO V. Tuning magnetic order in LSCO by a magnetic field SC+SDW SDW Néel

33
Superconductor with T c,min =10 K kyky kxkx /a 0 ~0.12-0.14 0.055 SC 0.020 J. M. Tranquada et al., Phys. Rev. B 54, 7489 (199 6). G. Aeppli, T.E. Mason, S.M. Hayden, H.A. Mook, J. Kulda, Science 278, 1432 (1997). S. Wakimoto, G. Shirane et al., Phys. Rev. B 60, R769 (1999). Y.S. Lee, R. J. Birgeneau, M. A. Kastner et al., Phys. Rev. B 60, 3643 (1999) S. Wakimoto, R.J. Birgeneau, Y.S. Lee, and G. Shirane, Phys. Rev. B 63, 172501 (2001). (additional commensurability effects near =0.125) T=0 phases of LSCO V. Tuning magnetic order in LSCO by a magnetic field SC+SDW SDW Néel

34
Spin density wave order Collinear spins

35
Superconductor with T c,min =10 K kyky kxkx /a 0 ~0.12-0.14 0.055 SC 0.020 T=0 phases of LSCO V. Tuning magnetic order in LSCO by a magnetic field SC+SDW SDW Néel Use simplest assumption of a direct second-order quantum phase transition between SC and SC+SDW phases

36
G. Aeppli, T.E. Mason, S,M. Hayden, H.A. Mook, and J. Kulda, Science 278, 1432 (1998).

37
Superconductor with T c,min =10 K kyky kxkx /a 0 ~0.12-0.14 0.055 SC 0.020 T=0 phases of LSCO V. Tuning magnetic order in LSCO by a magnetic field SC+SDW SDW Néel H Follow intensity of elastic Bragg spots in a magnetic field Use simplest assumption of a direct second-order quantum phase transition between SC and SC+SDW phases

38
H Spin singlet state SC+SDW Characteristic field g B H = , the spin gap 1 Tesla = 0.116 meV Effect is negligible over experimental field scales cc SC Zeeman term: only effect in coupled ladder system

39
uniform Dominant effect with coexisting superconductivity: uniform softening of spin excitations by superflow kinetic energy E. Demler, S. Sachdev, and Ying Zhang, Phys. Rev. Lett. 87, 067202 (2001). Competing order is enhanced in a “halo” around each vortex

40
Main results E. Demler, S. Sachdev, and Ying Zhang, Phys. Rev. Lett. 87, 067202 (2001). T=0 cc D. P. Arovas, A. J. Berlinsky, C. Kallin, and S.-C. Zhang, Phys. Rev. Lett. 79, 2871 (1997) proposed static local spins within vortex cores in SC phase “Normal” (Bond order)

41
Neutron scattering measurements of static spin correlations of the superconductor+spin-density-wave (SC+SDW) in a magnetic field H (Tesla)

42
B. Lake, H. M. Rønnow, N. B. Christensen, G. Aeppli, K. Lefmann, D. F. McMorrow, P. Vorderwisch, P. Smeibidl, N. Mangkorntong, T. Sasagawa, M. Nohara, H. Takagi, T. E. Mason, Nature, 415, 299 (2002). See also S. Katano, M. Sato, K. Yamada, T. Suzuki, and T. Fukase, Phys. Rev. B 62, R14677 (2000).

43
Neutron scattering observation of SDW order enhanced by superflow. cc Prediction: SDW fluctuations enhanced by superflow and bond order pinned by vortex cores (no spins in vortices). Should be observable in STM K. Park and S. Sachdev Phys. Rev. B 64, 184510 (2001). Y. Zhang, E. Demler and S. Sachdev, Phys. Rev. B 66, 094501 (2002). “Normal” (Bond order)

44
STM around vortices induced by a magnetic field in the superconducting state J. E. Hoffman, E. W. Hudson, K. M. Lang, V. Madhavan, S. H. Pan, H. Eisaki, S. Uchida, and J. C. Davis, Science 295, 466 (2002). Local density of states 1Å spatial resolution image of integrated LDOS of Bi 2 Sr 2 CaCu 2 O 8+ ( 1meV to 12 meV) at B=5 Tesla. S.H. Pan et al. Phys. Rev. Lett. 85, 1536 (2000).

45
100Å b 7 pA 0 pA Vortex-induced LDOS of Bi 2 Sr 2 CaCu 2 O 8+ integrated from 1meV to 12meV J. Hoffman E. W. Hudson, K. M. Lang, V. Madhavan, S. H. Pan, H. Eisaki, S. Uchida, and J. C. Davis, Science 295, 466 (2002).

46
Fourier Transform of Vortex-Induced LDOS map J. Hoffman et al. Science, 295, 466 (2002). K-space locations of vortex induced LDOS Distances in k –space have units of 2 /a 0 a 0 =3.83 Å is Cu-Cu distance K-space locations of Bi and Cu atoms

47
Fourier Transform of Vortex-Induced LDOS map K-space locations of vortex induced LDOS Our interpretation: LDOS modulations are signals of bond order of period 4 revealed in vortex halo

48
C. Howald, H. Eisaki, N. Kaneko, and A. Kapitulnik, cond-mat/0201546 V. STM image of LDOS modulations in Bi 2 Sr 2 CaCu 2 O 8+ in zero magnetic field Period = 4 lattice spacings

49
C. Howald, H. Eisaki, N. Kaneko, and A. Kapitulnik, cond-mat/0201546 Spectral properties of the STM signal are sensitive to the microstructure of the charge order Measured energy dependence of the Fourier component of the density of states which modulates with a period of 4 lattice spacings M. Vojta, Phys. Rev. B 66, 104505 (2002); D. Podolsky, E. Demler, K. Damle, and B.I. Halperin, cond-mat/0204011 Theoretical modeling shows that this spectrum is best obtained by a modulation of bond variables, such as the exchange, kinetic or pairing energies.

50
Global phase diagram M. Vojta and S. Sachdev, Phys. Rev. Lett. 83, 3916 (1999) M. Vojta, Y. Zhang, and S. Sachdev, Phys. Rev. B 62, 6721 (2000). M. Vojta, Phys. Rev. B 66, 104505 (2002);. See also J. Zaanen, Physica C 217, 317 (1999), V.J. Emery, S.A. Kivelson, and H.Q. Lin, Phys. Rev. Lett. 64, 475 (1990). S. White and D. Scalapino, Phys. Rev. Lett. 80, 1272 (1998). C. Castellani, C. Di Castro, and M. Grilli, Phys.Rev. Lett. 75, 4650 (1995). S. Mazumdar, R.T. Clay, and D.K. Campbell, Phys. Rev. B 62, 13400 (2000). Collinear magnetic order Bond order Neutrons STM

51
Conclusions I.Cuprate superconductivity is associated with doping Mott insulators with charge carriers. II.Order parameters characterizing the Mott insulator compete with the order associated with the Bose-Einstein condensation of Cooper pairs. III.Classification of Mott insulators shows that the appropriate order parameters are collinear magnetism and bond order. IV.Theory of quantum phase transitions provides semi- quantitative predictions for neutron scattering measurements of spin-density-wave order in superconductors; theory also proposes a connection to STM experiments. V.Future experiments should search for SC+SDW to SC quantum transition driven by a magnetic field. Conclusions I.Cuprate superconductivity is associated with doping Mott insulators with charge carriers. II.Order parameters characterizing the Mott insulator compete with the order associated with the Bose-Einstein condensation of Cooper pairs. III.Classification of Mott insulators shows that the appropriate order parameters are collinear magnetism and bond order. IV.Theory of quantum phase transitions provides semi- quantitative predictions for neutron scattering measurements of spin-density-wave order in superconductors; theory also proposes a connection to STM experiments. V.Future experiments should search for SC+SDW to SC quantum transition driven by a magnetic field.

Similar presentations

© 2019 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google